Low-Temperature Phase Transformation from Graphite to · PDF file 2011. 2. 22. ·...
Embed Size (px)
Transcript of Low-Temperature Phase Transformation from Graphite to · PDF file 2011. 2. 22. ·...
Low-Temperature Phase Transformation from Graphite to sp3 Orthorhombic Carbon
Jian-Tao Wang,1,2,* Changfeng Chen,2 and Yoshiyuki Kawazoe3
1Beijing National Laboratory for Condensed Matter Physics, Institute of Physics, Chinese Academy of Sciences, Beijing 100190, China
2Department of Physics and High Pressure Science and Engineering Center, University of Nevada, Las Vegas, Nevada 89154, USA 3Institute for Materials Research, Tohoku University, Sendai, 980-8577, Japan
(Received 17 November 2010; published 16 February 2011)
We identify by ab initio calculations an orthorhombic carbon polymorph in Pnma symmetry that has
the lowest enthalpy among proposed cold-compressed graphite phases. This new phase contains alter-
nating zigzag and armchair buckled carbon sheets transformed via a one-layer by three-layer slip
mechanism. It has a wide indirect band gap and a large bulk modulus that are comparable to those of
diamond. Its simulated x-ray diffraction pattern best matches the experimental data. Pressure plays a key
role in lowering the kinetic barrier during the phase conversion process. These results provide a
comprehensive understanding and an excellent account for experimental findings.
DOI: 10.1103/PhysRevLett.106.075501 PACS numbers: 61.50.Ks, 61.66.Bi, 62.50.�p, 63.20.D�
Carbon exhibits numerous phases with distinct sp2- and sp3-hybridized bonds . Without catalysts, graphite can be converted to hexagonal and cubic diamond at pressures above 15 GPa and temperatures above �1300 K [2–7]. Molecular dynamics studies  have shown that graphite layers first shift relative to one another under high pressure and then abruptly buckle, yielding a mixture of cubic and hexagonal diamonds. On the other hand, cold compression of graphite at room temperature produces a transparent and hard phase [9–15] distinct from hexagonal and cubic dia- mond. It is characterized by a marked increase in electrical resistivity from metal to insulator [9–13] above 15 GPa, an increase in optical transmittance above 18 GPa [9,10], a broadening of the higher frequency E2g Raman line ,
and changes in the x-ray diffraction (XRD) patterns above 14 GPa [11–14]. Recent theoretical studies have proposed several new structures for such cold-compressed graphite [16–18], including the monoclinic M carbon  and the body-centered tetragonal bct-C4 carbon . However, despite these findings, the atomistic mechanisms for the phase transformation and the lowest-enthalpy structural conversion paths remain largely unexplored .
In this Letter, we present a comprehensive study of the energetics and kinetics for the phase conversion of graphite under a wide pressure range of 5–25 GPa. We pay special attention to the initial reconstruction processes along vari- ous sliding and buckling pathways of the carbon sheets. We find that cold-compressed graphite tends to form an sp3-orthorhombic Pnma structure (named orthorhombic W carbon hereafter) with alternating zigzag and armchair buckled carbon sheets via a one-layer by three-layer slip mechanism. Throughout the conversion process, pressure plays a key role in lowering the kinetic barrier by establish- ing and maintaining energetically favorable bond recon- struction between carbon sheets. This new phase is more favorable than the previously proposed bct-C4 and
monoclinic M carbon in terms of both energetics (en- thalpy) and kinetics (enthalpy barrier), and also better matches the experimental x-ray diffraction pattern. The calculations were carried out using the density
functional theory within the local density approximation (LDA) as implemented in the Vienna ab initio simulation package (VASP) . The all-electron projector augmented wave (PAW) method  was adopted with 2s22p2 treated as valence electrons. A plane-wave basis set with an energy cutoff of 800 eV was used and gave well converged total energy of �1 meV per atom. Forces on the ions are calculated through the Hellmann-Feynman theorem allow- ing a full geometry optimization. The phase transitions are simulated using the climbing image nudged elastic band (CI NEB) method . Phonon calculations are performed using the package MedeA  with the forces calculated from VASP. We first characterize the structural, electronic, and me-
chanical properties of the new W carbon phase. Its crystal structure with the space group Pnma (D162h) is shown in Fig. 1(a). At zero pressure, the equilibrium lattice parame-
ters are a ¼ 8:979 �A, b ¼ 2:496 �A, and c ¼ 4:113 �A with four inequivalent crystallographic sites, occupying the 4c (0.1952, 0.75, 0.0755), (0.1895, 0.25, 0.3010), (0.5207, 0.25, 0.0914), and (0.4633, 0.25, 0.4316) positions, respec- tively. By fitting the calculated total energy as a function of volume to the third-order Birch-Murnaghan equation, we obtain the bulk modulus (B0) of W carbon as 444.5 GPa, which is larger than that of c-BN (396 GPa)  and very close to the value for diamond (466 GPa). At high pres- sures, W-carbon becomes stable relative to graphite above 12.32 GPa [Fig. 1(b)], and is more stable (i.e., lower in enthalpy) than both bct-C4 and M carbon. The electronic band structure of W carbon at 15 GPa is
shown in Fig. 1(c). The valence band top is at the � point and the conduction band bottom is at the T point. The LDA
PRL 106, 075501 (2011) P HY S I CA L R EV I EW LE T T E R S week ending
18 FEBRUARY 2011
0031-9007=11=106(7)=075501(4) 075501-1 � 2011 American Physical Society
band gap is 4.39–4.52 eVover a wide pressure range of 0– 25 GPa, which is remarkably larger than the value of 2.56 eV for bct C4  and 3.60 eV for M carbon ; it is even appreciably larger than the LDA gap (4.17 eV)  for diamond. Therefore, W carbon is expected to be opti- cally transparent in agreement with experiments .
We have calculated its phonon dispersion curves within a wide pressure range up to 40 GPa. No imaginary fre- quencies were observed throughout the whole Brillioun zone [results at 15 GPa are shown in Fig. 1(d)], confirming dynamical stability of the sp3-orthorhombic W carbon. The calculated volume, bulk modulus and band gaps at zero pressure are listed in Table I and compared to avail- able experimental data  for diamond and calculated data for bct-C4  and M carbon . These results provide an excellent account for the transparent and super- hard cold-compressed graphite phase [1,14].
We now study the atomistic processes underlying the transformation from graphite toward the W carbon and other compressed phases. We have examined various sliding-buckling processes along the low-index orienta- tions  and  of graphite. The orthorhombic W-carbon is formed by alternating zigzag and armchair buckling via a one-layer (A1) by three-layer (B1,A2,B2) slip model along the  orientation [Fig. 2(a)]; M-carbon is formed by alternating zigzag and armchair buckling via a two-layer (A1,B1) by two-layer (A2,B2) slip model along the  orientation [Fig. 2(b)]; the bct-C4 phase is obtained by a one-layer (A1) by one-layer
(B1) slip model along the  orientation with armchair buckling [Fig. 2(c)]. For comparison, we also considered the pathways to form hexagonal diamond (hex-d) and cubic diamond (cub-d). Hex-d is obtained by a one-layer (A1) by one-layer (B1) slip model along the  orienta- tion via an orthorhombic configuration [Fig. 2(d)] with a
TABLE I. Calculated equilibrium volume (V0 in �A 3=atom),
bulk modulus (B0 in GPa) and band gaps (Eg in eV) for diamond,
bct-C4,M, andW carbon at zero pressure, compared to available experimental data  for diamond and calculated data for bct C4  and M carbon .
Structure Method V0 ( �A 3) B0 (GPa) Eg (eV)
Diamond this work 5.52 466.3 4.20
LDA  5.52 468.5
LDA  4.17
Exp  5.67 446 5.47
M carbon this work 5.79 438.7 3.56
LDA  5.78 431.2 3.60
bct C4 this work 5.83 433.7 2.58
LDA  5.82 428.7 2.56
W carbon this work 5.76 444.5 4.39
FIG. 1 (color online). Properties of the orthorhombic W car- bon in Pnma symmetry. (a) Polyhedral views of the crystal structure; (b) The enthalpy per atom for bct-C4 , M carbon , and W carbon as a function of pressure relative to graphite. (c) Calculated electronic band structure of W carbon at 15 GPa. (d) Calculated phonon dispersion curves of W carbon at 15 GPa.
FIG. 2 (color online). Pathways to form W carbon (a), M carbon (b), bct-C4 (c), hex-d (d), and cub-d (e) starting from graphite with distinct sliding-buckling processes of carbon sheets along the  or  orientations of graphite.
PRL 106, 075501 (2011) P HY S I CA L R EV I EW LE T T E R S week ending
18 FEBRUARY 2011
stacking different from that for bct-C4; cub-d is obtained by a two-layer (A1,B2) by two-layer (B1,A2) slip model along the  orientation with zigzag buckling [Fig. 2(e)] that is different than M or W carbon. Here the pathway to form hex-d with armchair buckling  is consistent with the experimental findings that the c axis of hex-d is per- pendicular to the original c axis of hex-g , and the pathway to form cub-d with zigzag buckling  leads to the final  diamond orientation parallel to the c axis of the hex-g, which is consistent with the results of shock-wave experiments . These pathways are simu- lated using the CI NEB method  with an 8-atom, or 16-atom supercell containing two carbon sheets for bct-C4, hex-d, or four carbon sheets for cub-d, M carbon, and W carbon. N